Electrochemical synthesis, characterisation and comparative ... Accepted... All experiments were...
Embed Size (px)
Transcript of Electrochemical synthesis, characterisation and comparative ... Accepted... All experiments were...
Electrochemical synthesis, characterisation and comparative study of new conducting polymers from amino-substituted naphthalene sulfonic acids
Alemnew Geto1,2 & Christopher M. A. Brett2
Received: 5 April 2016 /Revised: 10 July 2016 /Accepted: 17 July 2016 # Springer-Verlag Berlin Heidelberg 2016
Abstract Conducting polymers have been synthesised elec- trochemically from 4-amino-3-hydroxynaphthalene-1-sulfon- ic acid (4A3HN1SA), 4-aminonaphthalene-1-sulfonic acid (4AN1SA) and 7-amino-4-hydroxynaphthalene-2-sulfonic acid (7A4HN2SA) on glassy carbon electrodes. The influence of the positive potential limit on the potential cycling poly- merisation of 4A3HN1SAwas studied, and a sufficiently high potential limit allowed better film growth. Under similar po- lymerisation conditions, the three monomers showed different radical formation potentials and different voltammetric peak profiles. The effects of scan rate and solution pH on the elec- trochemical properties of the polymers were investigated, in the range between 10 and 200 mV s−1, all the modified elec- trodes showing a surface-confined electrode process. In the pH range from 2.0 to 9.0, the anodic peak potentials decreased linearly with increasing pH for all the three modified elec- trodes. The modified electrodes were characterised by electro- chemical impedance spectroscopy in pH 4.0 and 7.0 buffer s o l u t i on s . The r e su l t s s howed a more po rou s poly(7A4HN2SA) film, which is less affected by pH change than the other two films. Scanning electron microscopy of the polymer films also showed significant differences in their morphologies.
Keywords Conducting polymer . Amino-naphthalene sulfonic acid . Electropolymerisation . Electrochemical impedance spectroscopy .Morphology . Polymer-modified electrodes
Since their discovery, conducting polymers have attracted global attention in both research and industrial applications. The possibility of finding the combined properties of process- ability and flexibility of organic polymers and electronic prop- erties of semiconductors and conductors in these materials is the main driving force for various applications . Furthermore, their properties can be tailored electrochemical- ly, mechanically, chemically and biochemically to suit specific applications, e.g. .
Among the conducting polymers, extensive work has been devoted to the study of only a few classes, such as polypyr- role, polyaniline, polythiophene and their derivatives . However, recent trends show increasing interest in fused ring systems such as polynaphthalenes and their derivatives, owing to their remarkable inherent properties such as intense fluores- cence, non-linear optical properties, strong π-stacking and good chemical stability. Such properties of naphthalene- based polymers and their derivatives allow the prospect of a considerable range of applications in various domains such as chemical sensors [4–11], batteries , electrochromic and electroluminescence devices [3, 13–16] and anti-corrosion coatings [17–21].
However, most of the reports to date have focused on co- polymers [6, 17, 21–23] or composites [7, 8, 12] which utilise naphthalenes or their substituted derivatives as one compo- nent. The use of naphthalenes and their derivatives in co- polymers and composites was found to impart uniformity
* Christopher M. A. Brett email@example.com
1 Department of Chemistry, School of Natural and Computational Sciences, Samara University, Samara, Ethiopia
2 Department of Chemistry, Faculty of Sciences and Technology, University of Coimbra, 3004-535 Coimbra, Portugal
J Solid State Electrochem DOI 10.1007/s10008-016-3338-9
and stability to the polymer films , increase the selectivity  and catalytic activity  of chemical sensors, enhance corrosion protection efficiency , increase polymer pro- cessability  and surface reactivity .
Although some naphthalenes and their derivatives have been known for a long time to undergo homopolymerisation and co-polymerisation by both chemical and electrochemical routes, reports on their homopolymers are still limited. Hence, the synthesis and characterisation of homopolymers with high-quality and improved properties is needed and essential owing to their simplicity and potential use for new applica- tions .
The polymerisation and applicability of 4-amino-3- hydroxynaphthalene-1-sulfonic acid has previously been demonstrated in the catalytic reduction of oxygen , anti- corrosion coatings [17, 20] and electrochemical determination of some biologically important compounds [8–10]. These re- ports showed excellent performance of the polymer film that served as a stable catalytic layer in modified electrodes and as an efficient corrosion inhibitor of different materials.
The monomer 4-amino-3-hydroxynaphthalene-1-sulfonic acid contains amino (–NH2), hydroxyl (–OH) and sulfonic acid (–SO3H) functional groups in its structure. The presence of such functional groups in monomers and their existence in the resulting polymer backbone plays an important role in various applications . For instance, the existence of sul- fonic acid groups in polymer chains helps to improve the solubility of the polymers in common polar solvents [19, 24]. Moreover, the polymers acquire an intrinsic proton dop- ing ability leading to the formation of highly soluble self- doped homopolymers and co-polymers . On the contrary, the extra benzene ring on substituted naphthalene molecules would confer greater hydrophobicity to the films formed from these materials (compared with their substituted benzene counterparts). It could also result in a lower degree of solva- tion, closer packing of the polymer chains, and reduced diffu- sion of solvated species through the film .
In addition, the presence of free –OH and –NH2 in the polymer chain helps to promote attachment to other functional groups which can give the polymer film strong binding prop- erties and good compatibility with other polymer layers and underlying surfaces .
In this work, the electrochemical potentiodynamic poly- merisation of 4-amino-3-hydroxynaphthalene-1-sulfonic acid (4A3HN1SA) is investigated using different potential ranges and supporting electrolyte media. The optimum condition is then extended to polymerise and study the structurally similar monomers, 7-amino-4-hydroxynaphthalene-2-sulfonic acid (7A4HN2SA) and 4-aminonaphthalene-1-sulfonic acid (4AN1SA) (Fig. 1). After electrochemical polymerisation, the resulting polymer films from the three monomers were characterised by cyclic voltammetry, electrochemical imped- ance spectroscopy and scanning electron microscopy. To the
best of our knowledge, the polymerisation and characterisa- tion of 7-amino-4-hydroxynaphthalene-2-sulfonic acid and 4- aminonaphthalene-1-sulfonic acid has not been reported previously.
Reagents and solutions
The monomers 4-amino-3-hydroxynaphthalene-1-sulfonic acid (4A3HN1SA), 4-aminonaphthalene-1-sulfonic acid (4AN1SA) and 7-amino-4-hydroxynaphthalene-2-sulfonic acid (7A4HN2SA) were purchased from Sigma-Aldrich. Britton-Robinson (B-R) buffer solutions were prepared from a mixture of boric acid (May and Baker Ltd.), acetic acid (Fischer Scientific Ltd.), 85 % phosphoric acid (Riedel-de Haen AG) and NaOH (Riedel-de Haen GmbH).
All chemicals were analytical reagent grade and used as received without prior purification. All aqueous solutions were prepared with Millipore Milli-Q nanopure water (resis- tivity ≥18 MΩ cm). All experiments were performed at room temperature (25 ± 1 °C).
Electrochemical experiments were done using a potentiostat/ galvanostat (Autolab PGSTAT30) connected to a computer with General Purpose Electrochemical System software (GPES v4.9) and frequency analysis software (FRA v4.9) from Metrohm-Autolab (Utrecht, Netherlands).
Fig. 1 Chemical structures of 4-amino-3-hydroxynaphthalene-1- sulfonic acid (4A3HN1SA), 4-aminonaphthalene-1-sulfonic acid (4AN1SA) and 7-amino-4-hydroxynaphthalene-2-sulfonic acid (7A4HN2SA)
J Solid State Electrochem
All experiments were carried out in a three-electrode cell using a modified or unmodified glassy carbon working elec- trode (3 mm diameter), a platinum wire as counter electrode and a silver/silver chloride (Ag/AgCl, 3 M KCl) as reference electrode. For impedance experiments, a sinusoidal voltage perturbation of 10 mV was applied, scanning from 65 kHz to 0.1 Hz, with ten measurement points per frequency decade. The equivalent circuit modelling was done with ZView3.2 software (Scribner Associates, Inc., USA). The pH measure- ments were done with a CRISON 2001 micropH-meter (Spain).
Scanning electron microscopy (SEM) was performed on films deposited on indium tin oxide (ITO) electrodes of area about 1 cm2 with a Jeol JSM-5310 Scanning Microscope (JEOL, Inc., Peabody, MA, USA).
Prior to use, the glassy carbon electrode was polished with alumina powder and diamond spray of 1-μm diameter on a polishing cloth and thoroughly rinsed with ultrapure water (Milli-Q, Millipore).
The clean electrode was used to electropolymerise the re- spective monomer in a 0.1 M HNO3 supporting electrolyte solution containing 2 mM 4A3HN1SA, 4AN1SA or 7A4HN2SA. Polymer film deposition was followed by a stabilisation step in a monomer free 0.5 M H2SO4 solution by scanning the potential betw